Polyurea is a type of elastomer that is derived from the reaction product of an isocyanate component and a synthetic resin blend component through step-growth polymerization. The isocyanate can be aromatic or aliphatic in nature. It can be monomer, polymer, or any variant reaction of isocyanates, quasi-prepolymer or a prepolymer. The prepolymer, or quasi-prepolymer, can be made of an amine-terminated polymer resin, or a hydroxyl-terminated polymer resin.
The resin blend may be made up of amine-terminated polymer resins, and/or amine-terminated chain extenders. The amine-terminated polymer resins will not have any intentional hydroxyl moieties. Any hydroxyls are the result of incomplete conversion to the amine-terminated polymer resins. The resin blend may also contain additives, or non-primary components. These additives may contain hydroxyls, such as pre-dispersed pigments in a polyol carrier. Normally, the resin blend will not contain a catalyst(s).
Polymer structure 
The word polyurea is derived from the Greek words πολυ- - poly- meaning "many"; and ουρίας - oûron meaning "to urinate". The latter term refers to the substance urea, found in urine, rather than urine itself. Urea or carbamide is an organic compound with the chemical formula (NH2)2CO. The molecule has two amine groups (–NH2) joined by a carbonyl functional group (C=O). In a polyurea, alternating monomer units of isocyanates and amines react with each other to form urea linkages. Ureas can also be formed from the reaction of isocyanates and water which forms a carbamic acid intermediate. This acid quickly decomposes by splitting off carbon dioxide and leaving behind an amine. This amine then reacts with another isocyanate group to form the polyurea linkage. This two step reaction is used in what is commonly but improperly called polyurethane foams. The carbon dioxide that is liberated in this reaction is the primary blowing (foaming) agent especially in many polyurethane foams which more precisely should be called polyurethane/urea foams.
Development of two-component polyurethane and polyurea spray elastomers took place in the 1990s. Their fast reactivity and relative insensitivity to moisture make them useful coatings for large surface area projects, such as secondary containment, manhole and tunnel coatings, tank liners, and truck bed liners. Excellent adhesion to concrete and steel is obtained with the proper primer and surface treatment. They can also be used for spray molding and armor. Some polyureas reach strengths of 6000psi (40MPa) tensile and over 500% elongation making it a tough coating. The quick cure time allows many coats to be built up quickly.